##############################################################################
#                                                                            #
# This CIF contains the data in a paper accepted for publication in Journal  #
# of Applied Crystallography. It has been peer reviewed under the auspices   #
# of the IUCr Commission on Journals.                                        #
#                                                                            #
# Full details of the Crystallographic Information File format               #
# are given in the paper "The Crystallographic Information File (CIF):       #
# a New Standard Archive File for Crystallography" by S. R. Hall, F. H.      #
# Allen and I. D. Brown [Acta Cryst. (1991), A47, 655-685].                  #
#                                                                            #
# The current version of the core CIF dictionary may be obtained from        #
# ftp://ftp.iucr.org/pub/cif_core.dic. The current version number is 2.1.    #
#                                                                            #
# Software is freely available for graphical display of the structure(s) in  #
# this CIF.  For information consult the CIF home page http://www.iucr.org/  #
# cif/home.html                                                              #
#                                                                            #
#           Copyright International Union of Crystallography                 #
#                                                                            #
##############################################################################

data_ag2o3a
_audit_creation_method     SHELXL-97
_journal_date_recd_electronic     2003-08-04
_journal_date_accepted     2003-12-22
_journal_name_full     'Journal of Applied Crystallography'
_journal_year     2004
_journal_volume     37
_journal_issue      2
_journal_page_first     318
_journal_page_last     324
_journal_paper_category     FA
_chemical_name_systematic
;
 ?
;
_chemical_name_common     ?
_chemical_formula_moiety     ?
_chemical_formula_sum     'Ag7 Cl O12'
_chemical_formula_weight     982.54
_chemical_melting_point     ?
_symmetry_cell_setting     Cubic
_symmetry_space_group_name_H-M     Fm-3m
loop_
    _symmetry_equiv_pos_as_xyz
    'x, y, z'
    '-x, -y, z'
    '-x, y, -z'
    'x, -y, -z'
    'z, x, y'
    'z, -x, -y'
    '-z, -x, y'
    '-z, x, -y'
    'y, z, x'
    '-y, z, -x'
    'y, -z, -x'
    '-y, -z, x'
    'y, x, -z'
    '-y, -x, -z'
    'y, -x, z'
    '-y, x, z'
    'x, z, -y'
    '-x, z, y'
    '-x, -z, -y'
    'x, -z, y'
    'z, y, -x'
    'z, -y, x'
    '-z, y, x'
    '-z, -y, -x'
    'x, y+1/2, z+1/2'
    '-x, -y+1/2, z+1/2'
    '-x, y+1/2, -z+1/2'
    'x, -y+1/2, -z+1/2'
    'z, x+1/2, y+1/2'
    'z, -x+1/2, -y+1/2'
    '-z, -x+1/2, y+1/2'
    '-z, x+1/2, -y+1/2'
    'y, z+1/2, x+1/2'
    '-y, z+1/2, -x+1/2'
    'y, -z+1/2, -x+1/2'
    '-y, -z+1/2, x+1/2'
    'y, x+1/2, -z+1/2'
    '-y, -x+1/2, -z+1/2'
    'y, -x+1/2, z+1/2'
    '-y, x+1/2, z+1/2'
    'x, z+1/2, -y+1/2'
    '-x, z+1/2, y+1/2'
    '-x, -z+1/2, -y+1/2'
    'x, -z+1/2, y+1/2'
    'z, y+1/2, -x+1/2'
    'z, -y+1/2, x+1/2'
    '-z, y+1/2, x+1/2'
    '-z, -y+1/2, -x+1/2'
    'x+1/2, y, z+1/2'
    '-x+1/2, -y, z+1/2'
    '-x+1/2, y, -z+1/2'
    'x+1/2, -y, -z+1/2'
    'z+1/2, x, y+1/2'
    'z+1/2, -x, -y+1/2'
    '-z+1/2, -x, y+1/2'
    '-z+1/2, x, -y+1/2'
    'y+1/2, z, x+1/2'
    '-y+1/2, z, -x+1/2'
    'y+1/2, -z, -x+1/2'
    '-y+1/2, -z, x+1/2'
    'y+1/2, x, -z+1/2'
    '-y+1/2, -x, -z+1/2'
    'y+1/2, -x, z+1/2'
    '-y+1/2, x, z+1/2'
    'x+1/2, z, -y+1/2'
    '-x+1/2, z, y+1/2'
    '-x+1/2, -z, -y+1/2'
    'x+1/2, -z, y+1/2'
    'z+1/2, y, -x+1/2'
    'z+1/2, -y, x+1/2'
    '-z+1/2, y, x+1/2'
    '-z+1/2, -y, -x+1/2'
    'x+1/2, y+1/2, z'
    '-x+1/2, -y+1/2, z'
    '-x+1/2, y+1/2, -z'
    'x+1/2, -y+1/2, -z'
    'z+1/2, x+1/2, y'
    'z+1/2, -x+1/2, -y'
    '-z+1/2, -x+1/2, y'
    '-z+1/2, x+1/2, -y'
    'y+1/2, z+1/2, x'
    '-y+1/2, z+1/2, -x'
    'y+1/2, -z+1/2, -x'
    '-y+1/2, -z+1/2, x'
    'y+1/2, x+1/2, -z'
    '-y+1/2, -x+1/2, -z'
    'y+1/2, -x+1/2, z'
    '-y+1/2, x+1/2, z'
    'x+1/2, z+1/2, -y'
    '-x+1/2, z+1/2, y'
    '-x+1/2, -z+1/2, -y'
    'x+1/2, -z+1/2, y'
    'z+1/2, y+1/2, -x'
    'z+1/2, -y+1/2, x'
    '-z+1/2, y+1/2, x'
    '-z+1/2, -y+1/2, -x'
    '-x, -y, -z'
    'x, y, -z'
    'x, -y, z'
    '-x, y, z'
    '-z, -x, -y'
    '-z, x, y'
    'z, x, -y'
    'z, -x, y'
    '-y, -z, -x'
    'y, -z, x'
    '-y, z, x'
    'y, z, -x'
    '-y, -x, z'
    'y, x, z'
    '-y, x, -z'
    'y, -x, -z'
    '-x, -z, y'
    'x, -z, -y'
    'x, z, y'
    '-x, z, -y'
    '-z, -y, x'
    '-z, y, -x'
    'z, -y, -x'
    'z, y, x'
    '-x, -y+1/2, -z+1/2'
    'x, y+1/2, -z+1/2'
    'x, -y+1/2, z+1/2'
    '-x, y+1/2, z+1/2'
    '-z, -x+1/2, -y+1/2'
    '-z, x+1/2, y+1/2'
    'z, x+1/2, -y+1/2'
    'z, -x+1/2, y+1/2'
    '-y, -z+1/2, -x+1/2'
    'y, -z+1/2, x+1/2'
    '-y, z+1/2, x+1/2'
    'y, z+1/2, -x+1/2'
    '-y, -x+1/2, z+1/2'
    'y, x+1/2, z+1/2'
    '-y, x+1/2, -z+1/2'
    'y, -x+1/2, -z+1/2'
    '-x, -z+1/2, y+1/2'
    'x, -z+1/2, -y+1/2'
    'x, z+1/2, y+1/2'
    '-x, z+1/2, -y+1/2'
    '-z, -y+1/2, x+1/2'
    '-z, y+1/2, -x+1/2'
    'z, -y+1/2, -x+1/2'
    'z, y+1/2, x+1/2'
    '-x+1/2, -y, -z+1/2'
    'x+1/2, y, -z+1/2'
    'x+1/2, -y, z+1/2'
    '-x+1/2, y, z+1/2'
    '-z+1/2, -x, -y+1/2'
    '-z+1/2, x, y+1/2'
    'z+1/2, x, -y+1/2'
    'z+1/2, -x, y+1/2'
    '-y+1/2, -z, -x+1/2'
    'y+1/2, -z, x+1/2'
    '-y+1/2, z, x+1/2'
    'y+1/2, z, -x+1/2'
    '-y+1/2, -x, z+1/2'
    'y+1/2, x, z+1/2'
    '-y+1/2, x, -z+1/2'
    'y+1/2, -x, -z+1/2'
    '-x+1/2, -z, y+1/2'
    'x+1/2, -z, -y+1/2'
    'x+1/2, z, y+1/2'
    '-x+1/2, z, -y+1/2'
    '-z+1/2, -y, x+1/2'
    '-z+1/2, y, -x+1/2'
    'z+1/2, -y, -x+1/2'
    'z+1/2, y, x+1/2'
    '-x+1/2, -y+1/2, -z'
    'x+1/2, y+1/2, -z'
    'x+1/2, -y+1/2, z'
    '-x+1/2, y+1/2, z'
    '-z+1/2, -x+1/2, -y'
    '-z+1/2, x+1/2, y'
    'z+1/2, x+1/2, -y'
    'z+1/2, -x+1/2, y'
    '-y+1/2, -z+1/2, -x'
    'y+1/2, -z+1/2, x'
    '-y+1/2, z+1/2, x'
    'y+1/2, z+1/2, -x'
    '-y+1/2, -x+1/2, z'
    'y+1/2, x+1/2, z'
    '-y+1/2, x+1/2, -z'
    'y+1/2, -x+1/2, -z'
    '-x+1/2, -z+1/2, y'
    'x+1/2, -z+1/2, -y'
    'x+1/2, z+1/2, y'
    '-x+1/2, z+1/2, -y'
    '-z+1/2, -y+1/2, x'
    '-z+1/2, y+1/2, -x'
    'z+1/2, -y+1/2, -x'
    'z+1/2, y+1/2, x'
_cell_length_a     9.955(6)
_cell_length_b     9.955(6)
_cell_length_c     9.955(6)
_cell_angle_alpha     90.00
_cell_angle_beta     90.00
_cell_angle_gamma     90.00
_cell_volume     986.5(10)
_cell_formula_units_Z     4
_cell_measurement_reflns_used     928
_cell_measurement_theta_min     8.2
_cell_measurement_theta_max     29.7
_cell_measurement_temperature     293(2)
_exptl_crystal_description     block
_exptl_crystal_colour     Black
_exptl_crystal_size_max     0.05
_exptl_crystal_size_mid     0.05
_exptl_crystal_size_min     0.05
_exptl_crystal_density_diffrn     6.615
_exptl_crystal_density_meas     ?
_exptl_crystal_density_method     'not measured'
_exptl_crystal_F_000     1768
_exptl_absorpt_coefficient_mu     13.943
_exptl_absorpt_correction_type     Multi-scan
_exptl_absorpt_process_details     ?
_exptl_absorpt_correction_T_min     0.577
_exptl_absorpt_correction_T_max     1.000
_exptl_special_details
;
 ?
;
_diffrn_ambient_temperature     293(2)
_diffrn_radiation_type     MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_source     'fine-focus sealed tube'
_diffrn_radiation_monochromator     graphite
_diffrn_measurement_device_type     'Bruker Smart APEX'
_diffrn_measurement_method     Omega
_diffrn_detector_area_resol_mean     ?
_diffrn_reflns_number     1447
_diffrn_reflns_av_R_equivalents     0.0209
_diffrn_reflns_av_sigmaI/netI     0.0114
_diffrn_reflns_theta_min     8.21
_diffrn_reflns_theta_max     30.57
_diffrn_reflns_theta_full     30.57
_diffrn_measured_fraction_theta_max     0.917
_diffrn_measured_fraction_theta_full     0.917
_diffrn_reflns_limit_h_min     -13
_diffrn_reflns_limit_h_max     10
_diffrn_reflns_limit_k_min     -14
_diffrn_reflns_limit_k_max     13
_diffrn_reflns_limit_l_min     -13
_diffrn_reflns_limit_l_max     12
_diffrn_standards_number     ?
_diffrn_standards_interval_count     ?
_diffrn_standards_interval_time     ?
_diffrn_standards_decay_%     ?
_refine_special_details
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;
_reflns_number_total     99
_reflns_number_gt     98
_reflns_threshold_expression     >2sigma(I)
_refine_ls_structure_factor_coef     Fsqd
_refine_ls_matrix_type     full
_refine_ls_R_factor_all     0.0216
_refine_ls_R_factor_gt     0.0214
_refine_ls_wR_factor_gt     0.0623
_refine_ls_wR_factor_ref     0.0625
_refine_ls_goodness_of_fit_ref     1.181
_refine_ls_restrained_S_all     1.181
_refine_ls_number_reflns     99
_refine_ls_number_parameters     9
_refine_ls_number_restraints     0
_refine_ls_hydrogen_treatment     n/a
_refine_ls_weighting_scheme     calc
_refine_ls_weighting_details
        'calc w=1/[σ²(Fo²)+(0.0279P)²+17.3641P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_hydrogens     n/a
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary     difmap
_refine_ls_shift/su_max     0.000
_refine_ls_shift/su_mean     0.000
_refine_diff_density_max     1.527
_refine_diff_density_min     -0.864
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef     0.00119(14)
_refine_ls_extinction_expression
                                  'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^'
loop_
    _atom_type_symbol
    _atom_type_description
    _atom_type_scat_dispersion_real
    _atom_type_scat_dispersion_imag
    _atom_type_scat_source
    'O' 'O' 0.0106 0.0060
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
    'Cl' 'Cl' 0.1484 0.1585
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
    'Ag' 'Ag' -0.8971 1.1015
                         'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
_computing_data_collection     ?
_computing_cell_refinement     ?
_computing_data_reduction     ?
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement     'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics     ?
_computing_publication_material     ?
loop_
    _atom_site_label
    _atom_site_fract_x
    _atom_site_fract_y
    _atom_site_fract_z
    _atom_site_U_iso_or_equiv
    _atom_site_adp_type
    _atom_site_calc_flag
    _atom_site_refinement_flags
    _atom_site_occupancy
    _atom_site_disorder_assembly
    _atom_site_disorder_group
    _atom_site_type_symbol
    Ag1 0.0000 0.5000 0.0000 0.0128(4) Uani d S 1 . . Ag
    Ag2 0.0000 0.7500 -0.2500 0.0134(4) Uani d S 1 . . Ag
    O1 0.1406(3) 0.6406(3) -0.1406(3) 0.0195(10) Uani d S 1 . . O
    Cl1 0.0000 0.5000 -0.5000 0.050 Uiso d S 1 . . Cl
    O2 0.0000 0.5000 -0.6410 0.060 Uiso d SP 0.17 . . O
    O3 0.0000 0.6330 -0.4530 0.060 Uiso d SP 0.04 . . O
    O4 0.1150 0.4340 -0.4530 0.060 Uiso d P 0.04 . . O
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
    _geom_bond_atom_site_label_1
    _geom_bond_atom_site_label_2
    _geom_bond_site_symmetry_2
    _geom_bond_distance
    _geom_bond_publ_flag
    Ag1 O1 98 2.424(5) ?
    Ag1 O1 2_565 2.424(5) ?
    Ag1 O1 100 2.424(5) ?
    Ag1 O1 97_565 2.424(5) ?
    Ag1 O1 4_565 2.424(5) ?
    Ag1 O1 3 2.424(5) ?
    Ag1 O1 99_565 2.424(5) ?
    Ag1 O1 . 2.424(5) ?
    Ag2 O1 100 2.0812(17) ?
    Ag2 O1 28_564 2.0812(17) ?
    Ag2 O1 121_564 2.0812(17) ?
    Ag2 O1 . 2.0812(17) ?
    Ag2 O4 165_464 2.3195 ?
    Ag2 O4 93 2.3195 ?
    Ag2 O4 152_564 2.3195 ?
    Ag2 O4 80_455 2.3195 ?
    Ag2 O4 190_455 2.3195 ?
    Ag2 O4 55_464 2.3195 ?
    Ag2 O4 175 2.3195 ?
    Ag2 O4 70_564 2.3195 ?
    O1 Ag2 10_665 2.0812(17) ?
    O1 Ag2 77_554 2.0812(17) ?
    Cl1 O4 166_454 1.4004 ?
    Cl1 O4 70_564 1.4004 ?
    Cl1 O4 113_554 1.4004 ?
    Cl1 O4 17_565 1.4004 ?
    Cl1 O4 184_454 1.4004 ?
    Cl1 O4 88 1.4004 ?
    Cl1 O4 155_564 1.4004 ?
    Cl1 O4 59_454 1.4004 ?
    Cl1 O4 175 1.4004 ?
    Cl1 O4 79_454 1.4004 ?
    Cl1 O4 99_565 1.4004 ?
    Cl1 O4 3_554 1.4004 ?
    O2 O3 17_565 0.4746 ?
    O2 O3 78 0.4746 ?
    O2 O3 114 0.4746 ?
    O2 O3 173_455 0.4746 ?
    O2 O4 167_564 0.8471 ?
    O2 O4 58_564 0.8471 ?
    O2 O4 166_454 0.8471 ?
    O2 O4 59_454 0.8471 ?
    O2 O4 72_464 0.8471 ?
    O2 O4 153_554 0.8471 ?
    O2 O4 69_554 0.8471 ?
    O2 O4 156_464 0.8471 ?
    O3 O2 153_554 0.4746 ?
    O3 O4 175 0.5355 ?
    O3 O4 80_455 0.5355 ?
    O3 O3 166_454 0.6617 ?
    O3 O3 69_554 0.6617 ?
    O3 O4 182_455 0.6810 ?
    O3 O4 88 0.6810 ?
    O3 O3 98_554 0.9358 ?
    O3 O4 70_564 1.0592 ?
    O3 O4 165_464 1.0592 ?
    O3 O4 85_454 1.1573 ?
    O3 O4 183_554 1.1573 ?
    O4 O4 114 0.2675 ?
    O4 O3 154_454 0.5355 ?
    O4 O3 182_455 0.6810 ?
    O4 O4 181 0.6898 ?
    O4 O2 173_455 0.8471 ?
    O4 O4 60_554 0.8555 ?
    O4 O4 78 0.8555 ?
    O4 O4 98_554 0.9358 ?
    O4 O4 168_554 0.9573 ?
    O4 O3 70_564 1.0593 ?
    O4 O4 17_565 1.1407 ?
    O4 O4 20_554 1.1407 ?
loop_
    _geom_angle_atom_site_label_1
    _geom_angle_atom_site_label_2
    _geom_angle_atom_site_label_3
    _geom_angle_site_symmetry_1
    _geom_angle_site_symmetry_3
    _geom_angle
    _geom_angle_publ_flag
    O1 Ag1 O1 98 2_565 180.0 ?
    O1 Ag1 O1 98 100 109.5 ?
    O1 Ag1 O1 2_565 100 70.5 ?
    O1 Ag1 O1 98 97_565 109.5 ?
    O1 Ag1 O1 2_565 97_565 70.5 ?
    O1 Ag1 O1 100 97_565 109.5 ?
    O1 Ag1 O1 98 4_565 70.5 ?
    O1 Ag1 O1 2_565 4_565 109.5 ?
    O1 Ag1 O1 100 4_565 180.00(12) ?
    O1 Ag1 O1 97_565 4_565 70.5 ?
    O1 Ag1 O1 98 3 70.5 ?
    O1 Ag1 O1 2_565 3 109.5 ?
    O1 Ag1 O1 100 3 70.5 ?
    O1 Ag1 O1 97_565 3 70.5 ?
    O1 Ag1 O1 4_565 3 109.5 ?
    O1 Ag1 O1 98 99_565 109.4710(10)
                                   ?
    O1 Ag1 O1 2_565 99_565 70.5 ?
    O1 Ag1 O1 100 99_565 109.5 ?
    O1 Ag1 O1 97_565 99_565 109.5 ?
    O1 Ag1 O1 4_565 99_565 70.5 ?
    O1 Ag1 O1 3 99_565 180.0 ?
    O1 Ag1 O1 98 . 70.5 ?
    O1 Ag1 O1 2_565 . 109.5 ?
    O1 Ag1 O1 100 . 70.5 ?
    O1 Ag1 O1 97_565 . 180.00(12) ?
    O1 Ag1 O1 4_565 . 109.5 ?
    O1 Ag1 O1 3 . 109.5 ?
    O1 Ag1 O1 99_565 . 70.5 ?
    O1 Ag2 O1 100 28_564 180.0 ?
    O1 Ag2 O1 100 121_564 95.5(3) ?
    O1 Ag2 O1 28_564 121_564 84.5(3) ?
    O1 Ag2 O1 100 . 84.5(3) ?
    O1 Ag2 O1 28_564 . 95.5(3) ?
    O1 Ag2 O1 121_564 . 180.00(14) ?
    O1 Ag2 O4 100 165_464 75.777(7) ?
    O1 Ag2 O4 28_564 165_464 104.223(7) ?
    O1 Ag2 O4 121_564 165_464 88.53(3) ?
    O1 Ag2 O4 . 165_464 91.47(3) ?
    O1 Ag2 O4 100 93 104.223(7) ?
    O1 Ag2 O4 28_564 93 75.777(7) ?
    O1 Ag2 O4 121_564 93 91.47(3) ?
    O1 Ag2 O4 . 93 88.53(3) ?
    O4 Ag2 O4 165_464 93 180.0 ?
    O1 Ag2 O4 100 152_564 91.47(3) ?
    O1 Ag2 O4 28_564 152_564 88.53(3) ?
    O1 Ag2 O4 121_564 152_564 104.223(7) ?
    O1 Ag2 O4 . 152_564 75.777(7) ?
    O4 Ag2 O4 165_464 152_564 162.9 ?
    O4 Ag2 O4 93 152_564 17.1 ?
    O1 Ag2 O4 100 80_455 88.53(3) ?
    O1 Ag2 O4 28_564 80_455 91.47(3) ?
    O1 Ag2 O4 121_564 80_455 75.777(7) ?
    O1 Ag2 O4 . 80_455 104.223(7) ?
    O4 Ag2 O4 165_464 80_455 17.1 ?
    O4 Ag2 O4 93 80_455 162.9 ?
    O4 Ag2 O4 152_564 80_455 180.0 ?
    O1 Ag2 O4 100 190_455 88.53(3) ?
    O1 Ag2 O4 28_564 190_455 91.47(3) ?
    O1 Ag2 O4 121_564 190_455 75.777(7) ?
    O1 Ag2 O4 . 190_455 104.223(7) ?
    O4 Ag2 O4 165_464 190_455 156.7 ?
    O4 Ag2 O4 93 190_455 23.3 ?
    O4 Ag2 O4 152_564 190_455 29.0 ?
    O4 Ag2 O4 80_455 190_455 151.0 ?
    O1 Ag2 O4 100 55_464 75.777(7) ?
    O1 Ag2 O4 28_564 55_464 104.223(7) ?
    O1 Ag2 O4 121_564 55_464 88.53(3) ?
    O1 Ag2 O4 . 55_464 91.47(3) ?
    O4 Ag2 O4 165_464 55_464 151.0 ?
    O4 Ag2 O4 93 55_464 29.0 ?
    O4 Ag2 O4 152_564 55_464 23.3 ?
    O4 Ag2 O4 80_455 55_464 156.7 ?
    O4 Ag2 O4 190_455 55_464 17.1 ?
    O1 Ag2 O4 100 175 104.223(7) ?
    O1 Ag2 O4 28_564 175 75.777(7) ?
    O1 Ag2 O4 121_564 175 91.47(3) ?
    O1 Ag2 O4 . 175 88.53(3) ?
    O4 Ag2 O4 165_464 175 29.0 ?
    O4 Ag2 O4 93 175 151.0 ?
    O4 Ag2 O4 152_564 175 156.7 ?
    O4 Ag2 O4 80_455 175 23.3 ?
    O4 Ag2 O4 190_455 175 162.9 ?
    O4 Ag2 O4 55_464 175 180.0 ?
    O1 Ag2 O4 100 70_564 91.47(3) ?
    O1 Ag2 O4 28_564 70_564 88.53(3) ?
    O1 Ag2 O4 121_564 70_564 104.223(7) ?
    O1 Ag2 O4 . 70_564 75.777(7) ?
    O4 Ag2 O4 165_464 70_564 23.3 ?
    O4 Ag2 O4 93 70_564 156.7 ?
    O4 Ag2 O4 152_564 70_564 151.0 ?
    O4 Ag2 O4 80_455 70_564 29.0 ?
    O4 Ag2 O4 190_455 70_564 180.0 ?
    O4 Ag2 O4 55_464 70_564 162.9 ?
    O4 Ag2 O4 175 70_564 17.1 ?
    Ag2 O1 Ag2 10_665 . 115.46(10) ?
    Ag2 O1 Ag2 10_665 77_554 115.46(10) ?
    Ag2 O1 Ag2 . 77_554 115.46(10) ?
    Ag2 O1 Ag1 10_665 . 102.48(14) ?
    Ag2 O1 Ag1 . . 102.48(14) ?
    Ag2 O1 Ag1 77_554 . 102.48(14) ?
    O4 Cl1 O4 166_454 70_564 180.0 ?
    O4 Cl1 O4 166_454 113_554 35.6 ?
    O4 Cl1 O4 70_564 113_554 144.4 ?
    O4 Cl1 O4 166_454 17_565 144.4 ?
    O4 Cl1 O4 70_564 17_565 35.6 ?
    O4 Cl1 O4 113_554 17_565 180.0 ?
    O4 Cl1 O4 166_454 184_454 35.6 ?
    O4 Cl1 O4 70_564 184_454 144.4 ?
    O4 Cl1 O4 113_554 184_454 35.6 ?
    O4 Cl1 O4 17_565 184_454 144.4 ?
    O4 Cl1 O4 166_454 88 144.4 ?
    O4 Cl1 O4 70_564 88 35.6 ?
    O4 Cl1 O4 113_554 88 144.4 ?
    O4 Cl1 O4 17_565 88 35.6 ?
    O4 Cl1 O4 184_454 88 180.0 ?
    O4 Cl1 O4 166_454 155_564 169.0 ?
    O4 Cl1 O4 70_564 155_564 11.0 ?
    O4 Cl1 O4 113_554 155_564 151.5 ?
    O4 Cl1 O4 17_565 155_564 28.5 ?
    O4 Cl1 O4 184_454 155_564 140.0 ?
    O4 Cl1 O4 88 155_564 40.0 ?
    O4 Cl1 O4 166_454 59_454 11.0 ?
    O4 Cl1 O4 70_564 59_454 169.0 ?
    O4 Cl1 O4 113_554 59_454 28.5 ?
    O4 Cl1 O4 17_565 59_454 151.5 ?
    O4 Cl1 O4 184_454 59_454 40.0 ?
    O4 Cl1 O4 88 59_454 140.0 ?
    O4 Cl1 O4 155_564 59_454 180.0 ?
    O4 Cl1 O4 166_454 175 151.5 ?
    O4 Cl1 O4 70_564 175 28.5 ?
    O4 Cl1 O4 113_554 175 140.0 ?
    O4 Cl1 O4 17_565 175 40.0 ?
    O4 Cl1 O4 184_454 175 169.0 ?
    O4 Cl1 O4 88 175 11.0 ?
    O4 Cl1 O4 155_564 175 35.6 ?
    O4 Cl1 O4 59_454 175 144.4 ?
    O4 Cl1 O4 166_454 79_454 28.5 ?
    O4 Cl1 O4 70_564 79_454 151.5 ?
    O4 Cl1 O4 113_554 79_454 40.0 ?
    O4 Cl1 O4 17_565 79_454 140.0 ?
    O4 Cl1 O4 184_454 79_454 11.0 ?
    O4 Cl1 O4 88 79_454 169.0 ?
    O4 Cl1 O4 155_564 79_454 144.4 ?
    O4 Cl1 O4 59_454 79_454 35.6 ?
    O4 Cl1 O4 175 79_454 180.0 ?
    O4 Cl1 O4 166_454 99_565 140.0 ?
    O4 Cl1 O4 70_564 99_565 40.0 ?
    O4 Cl1 O4 113_554 99_565 169.0 ?
    O4 Cl1 O4 17_565 99_565 11.0 ?
    O4 Cl1 O4 184_454 99_565 151.5 ?
    O4 Cl1 O4 88 99_565 28.5 ?
    O4 Cl1 O4 155_564 99_565 35.6 ?
    O4 Cl1 O4 59_454 99_565 144.4 ?
    O4 Cl1 O4 175 99_565 35.6 ?
    O4 Cl1 O4 79_454 99_565 144.4 ?
    O4 Cl1 O4 166_454 3_554 40.0 ?
    O4 Cl1 O4 70_564 3_554 140.0 ?
    O4 Cl1 O4 113_554 3_554 11.0 ?
    O4 Cl1 O4 17_565 3_554 169.0 ?
    O4 Cl1 O4 184_454 3_554 28.5 ?
    O4 Cl1 O4 88 3_554 151.5 ?
    O4 Cl1 O4 155_564 3_554 144.4 ?
    O4 Cl1 O4 59_454 3_554 35.6 ?
    O4 Cl1 O4 175 3_554 144.4 ?
    O4 Cl1 O4 79_454 3_554 35.6 ?
    O4 Cl1 O4 99_565 3_554 180.0 ?
    O3 O2 O3 17_565 78 88.4 ?
    O3 O2 O3 17_565 114 160.7 ?
    O3 O2 O3 78 114 88.4 ?
    O3 O2 O3 17_565 173_455 88.4 ?
    O3 O2 O3 78 173_455 160.7 ?
    O3 O2 O3 114 173_455 88.4 ?
    O3 O2 O4 17_565 167_564 35.3 ?
    O3 O2 O4 78 167_564 53.4 ?
    O3 O2 O4 114 167_564 135.5 ?
    O3 O2 O4 173_455 167_564 119.6 ?
    O3 O2 O4 17_565 58_564 53.4 ?
    O3 O2 O4 78 58_564 35.3 ?
    O3 O2 O4 114 58_564 119.6 ?
    O3 O2 O4 173_455 58_564 135.5 ?
    O4 O2 O4 167_564 58_564 18.2 ?
    O3 O2 O4 17_565 166_454 135.5 ?
    O3 O2 O4 78 166_454 119.6 ?
    O3 O2 O4 114 166_454 35.3 ?
    O3 O2 O4 173_455 166_454 53.4 ?
    O4 O2 O4 167_564 166_454 144.4 ?
    O4 O2 O4 58_564 166_454 139.8 ?
    O3 O2 O4 17_565 59_454 119.6 ?
    O3 O2 O4 78 59_454 135.5 ?
    O3 O2 O4 114 59_454 53.4 ?
    O3 O2 O4 173_455 59_454 35.3 ?
    O4 O2 O4 167_564 59_454 139.8 ?
    O4 O2 O4 58_564 59_454 144.4 ?
    O4 O2 O4 166_454 59_454 18.2 ?
    O3 O2 O4 17_565 72_464 35.3 ?
    O3 O2 O4 78 72_464 119.6 ?
    O3 O2 O4 114 72_464 135.5 ?
    O3 O2 O4 173_455 72_464 53.4 ?
    O4 O2 O4 167_564 72_464 67.1 ?
    O4 O2 O4 58_564 72_464 84.6 ?
    O4 O2 O4 166_454 72_464 101.7 ?
    O4 O2 O4 59_454 72_464 84.6 ?
    O3 O2 O4 17_565 153_554 119.6 ?
    O3 O2 O4 78 153_554 35.3 ?
    O3 O2 O4 114 153_554 53.4 ?
    O3 O2 O4 173_455 153_554 135.5 ?
    O4 O2 O4 167_564 153_554 84.6 ?
    O4 O2 O4 58_564 153_554 67.1 ?
    O4 O2 O4 166_454 153_554 84.6 ?
    O4 O2 O4 59_454 153_554 101.7 ?
    O4 O2 O4 72_464 153_554 139.8 ?
    O3 O2 O4 17_565 69_554 135.5 ?
    O3 O2 O4 78 69_554 53.4 ?
    O3 O2 O4 114 69_554 35.3 ?
    O3 O2 O4 173_455 69_554 119.6 ?
    O4 O2 O4 167_564 69_554 101.7 ?
    O4 O2 O4 58_564 69_554 84.6 ?
    O4 O2 O4 166_454 69_554 67.1 ?
    O4 O2 O4 59_454 69_554 84.6 ?
    O4 O2 O4 72_464 69_554 144.4 ?
    O4 O2 O4 153_554 69_554 18.2 ?
    O3 O2 O4 17_565 156_464 53.4 ?
    O3 O2 O4 78 156_464 135.5 ?
    O3 O2 O4 114 156_464 119.6 ?
    O3 O2 O4 173_455 156_464 35.3 ?
    O4 O2 O4 167_564 156_464 84.6 ?
    O4 O2 O4 58_564 156_464 101.7 ?
    O4 O2 O4 166_454 156_464 84.6 ?
    O4 O2 O4 59_454 156_464 67.1 ?
    O4 O2 O4 72_464 156_464 18.2 ?
    O4 O2 O4 153_554 156_464 144.4 ?
    O4 O2 O4 69_554 156_464 139.8 ?
    O2 O3 O4 153_554 175 113.8 ?
    O2 O3 O4 153_554 80_455 113.8 ?
    O4 O3 O4 175 80_455 121.8 ?
    O2 O3 O3 153_554 166_454 45.8 ?
    O4 O3 O3 175 166_454 150.2 ?
    O4 O3 O3 80_455 166_454 68.4 ?
    O2 O3 O3 153_554 69_554 45.8 ?
    O4 O3 O3 175 69_554 68.4 ?
    O4 O3 O3 80_455 69_554 150.2 ?
    O3 O3 O3 166_454 69_554 90.0 ?
    O2 O3 O4 153_554 182_455 92.5 ?
    O4 O3 O4 175 182_455 139.0 ?
    O4 O3 O4 80_455 182_455 21.4 ?
    O3 O3 O4 166_454 182_455 47.0 ?
    O3 O3 O4 69_554 182_455 133.0 ?
    O2 O3 O4 153_554 88 92.5 ?
    O4 O3 O4 175 88 21.4 ?
    O4 O3 O4 80_455 88 139.0 ?
    O3 O3 O4 166_454 88 133.0 ?
    O3 O3 O4 69_554 88 47.0 ?
    O4 O3 O4 182_455 88 149.5 ?
    O2 O3 O3 153_554 98_554 9.7 ?
    O4 O3 O3 175 98_554 110.7 ?
    O4 O3 O3 80_455 98_554 110.7 ?
    O3 O3 O3 166_454 98_554 45.0 ?
    O3 O3 O3 69_554 98_554 45.0 ?
    O4 O3 O3 182_455 98_554 90.0 ?
    O4 O3 O3 88 98_554 90.0 ?
    O2 O3 O4 153_554 70_564 137.4 ?
    O4 O3 O4 175 70_564 34.7 ?
    O4 O3 O4 80_455 70_564 87.1 ?
    O3 O3 O4 166_454 70_564 139.8 ?
    O3 O3 O4 69_554 70_564 98.0 ?
    O4 O3 O4 182_455 70_564 105.1 ?
    O4 O3 O4 88 70_564 53.7 ?
    O3 O3 O4 98_554 70_564 129.7 ?
    O2 O3 O4 153_554 165_464 137.4 ?
    O4 O3 O4 175 165_464 87.1 ?
    O4 O3 O4 80_455 165_464 34.7 ?
    O3 O3 O4 166_454 165_464 98.0 ?
    O3 O3 O4 69_554 165_464 139.8 ?
    O4 O3 O4 182_455 165_464 53.7 ?
    O4 O3 O4 88 165_464 105.1 ?
    O3 O3 O4 98_554 165_464 129.7 ?
    O4 O3 O4 70_564 165_464 52.4 ?
    O2 O3 O4 153_554 85_454 39.5 ?
    O4 O3 O4 175 85_454 136.9 ?
    O4 O3 O4 80_455 85_454 74.8 ?
    O3 O3 O4 166_454 85_454 13.3 ?
    O3 O3 O4 69_554 85_454 80.2 ?
    O4 O3 O4 182_455 85_454 54.0 ?
    O4 O3 O4 88 85_454 120.5 ?
    O3 O3 O4 98_554 85_454 36.0 ?
    O4 O3 O4 70_564 85_454 132.1 ?
    O4 O3 O4 165_464 85_454 99.7 ?
    O2 O3 O4 153_554 183_554 39.5 ?
    O4 O3 O4 175 183_554 74.8 ?
    O4 O3 O4 80_455 183_554 136.9 ?
    O3 O3 O4 166_454 183_554 80.2 ?
    O3 O3 O4 69_554 183_554 13.3 ?
    O4 O3 O4 182_455 183_554 120.5 ?
    O4 O3 O4 88 183_554 54.0 ?
    O3 O3 O4 98_554 183_554 36.0 ?
    O4 O3 O4 70_564 183_554 99.7 ?
    O4 O3 O4 165_464 183_554 132.1 ?
    O4 O3 O4 85_454 183_554 69.2 ?
    O4 O4 O3 114 154_454 111.6 ?
    O4 O4 O3 114 182_455 47.0 ?
    O3 O4 O3 154_454 182_455 64.6 ?
    O4 O4 O4 114 181 120.0 ?
    O3 O4 O4 154_454 181 119.1 ?
    O3 O4 O4 182_455 181 150.3 ?
    O4 O4 O2 114 173_455 80.9 ?
    O3 O4 O2 154_454 173_455 30.8 ?
    O3 O4 O2 182_455 173_455 34.0 ?
    O4 O4 O2 181 173_455 139.9 ?
    O4 O4 O4 114 60_554 44.3 ?
    O3 O4 O4 154_454 60_554 143.5 ?
    O3 O4 O4 182_455 60_554 86.4 ?
    O4 O4 O4 181 60_554 75.7 ?
    O2 O4 O4 173_455 60_554 116.1 ?
    O4 O4 O4 114 78 104.3 ?
    O3 O4 O4 154_454 78 131.2 ?
    O3 O4 O4 182_455 78 139.3 ?
    O4 O4 O4 181 78 15.7 ?
    O2 O4 O4 173_455 78 143.7 ?
    O4 O4 O4 60_554 78 60.0 ?
    O4 O4 O4 114 98_554 135.0 ?
    O3 O4 O4 154_454 98_554 29.1 ?
    O3 O4 O4 182_455 98_554 90.0 ?
    O4 O4 O4 181 98_554 90.0 ?
    O2 O4 O4 173_455 98_554 56.5 ?
    O4 O4 O4 60_554 98_554 142.3 ?
    O4 O4 O4 78 98_554 102.8 ?
    O4 O4 O4 114 168_554 60.0 ?
    O3 O4 O4 154_454 168_554 148.7 ?
    O3 O4 O4 182_455 168_554 100.7 ?
    O4 O4 O4 181 168_554 60.0 ?
    O2 O4 O4 173_455 168_554 127.3 ?
    O4 O4 O4 60_554 168_554 15.7 ?
    O4 O4 O4 78 168_554 44.3 ?
    O4 O4 O4 98_554 168_554 135.0 ?
    O4 O4 O3 114 70_564 139.3 ?
    O3 O4 O3 154_454 70_564 92.9 ?
    O3 O4 O3 182_455 70_564 140.9 ?
    O4 O4 O3 181 70_564 26.2 ?
    O2 O4 O3 173_455 70_564 116.1 ?
    O4 O4 O3 60_554 70_564 97.1 ?
    O4 O4 O3 78 70_564 39.9 ?
    O4 O4 O3 98_554 70_564 63.8 ?
    O4 O4 O3 168_554 70_564 82.0 ?
    O4 O4 O4 114 17_565 35.5 ?
    O3 O4 O4 154_454 17_565 78.3 ?
    O3 O4 O4 182_455 17_565 17.9 ?
    O4 O4 O4 181 17_565 134.2 ?
    O2 O4 O4 173_455 17_565 47.7 ?
    O4 O4 O4 60_554 17_565 69.6 ?
    O4 O4 O4 78 17_565 121.7 ?
    O4 O4 O4 98_554 17_565 99.5 ?
    O4 O4 O4 168_554 17_565 83.3 ?
    O3 O4 O4 70_564 17_565 134.0 ?
    O4 O4 O4 114 20_554 125.5 ?
    O3 O4 O4 154_454 20_554 23.1 ?
    O3 O4 O4 182_455 20_554 80.8 ?
    O4 O4 O4 181 20_554 96.7 ?
    O2 O4 O4 173_455 20_554 47.7 ?
    O4 O4 O4 60_554 20_554 138.0 ?
    O4 O4 O4 78 20_554 108.2 ?
    O4 O4 O4 98_554 20_554 9.5 ?
    O4 O4 O4 168_554 20_554 134.2 ?
    O3 O4 O4 70_564 20_554 70.7 ?
    O4 O4 O4 17_565 20_554 90.0 ?
